FOR SOLIDS AND LIQUIDS. 



149 



Alloy. 



tin and lead — contin'd. 

 Sn Pb, 



Sn Pb, 



SnPb 4 



Sn Pb 5 

 Sn Pb K 



LEAD AND CADMIUM. 



Cd 6 Pb 

 Cd 4 Pb 

 Cd 2 Pb 

 Cd Pb. 

 Cd Pb, 

 Cd Pb 4 

 Cd Pb, 



ANTIMONY AND TIN. 



Sbj, Sn 



Sb 8 Sn 



Sb 4 Sn 



Sb 2 Sn 



SbSn 



Sb Sn 



Sb Sn 3 



BbSn. 



SbSn 10 



SbSn 20 



SbSn M __ 



SbSn inn 



ANTIMONY AND LEAD. 



Sb Pb 



Specific Gravity. 



9.966 



10.080, 14°.8__. 



10.105 



10.0520 



10.110 



10.3868 



10.421 



10.3311 



10.419 



10.5551 



10.590, 14°.3___ 



10.587 



10.5957 



10.751 



10.815, 15°.6__. 



9.160, 13°. 7.. 

 9.353, 12° __. 

 9.755, 14°.7_. 

 10.246, 110.7. 

 10.656, 13°.4. 

 10.950, 9°.2__ 

 11.044, 14°.8. 



6.739, 16°. 2. 

 6.747, 13.°4. 

 6.781, 18°.6_ 

 6.844, 18°.8_ 

 6.929, 15°.8. 

 7.023, 15°.8. 

 7.100, 10°.6. 

 7.140, 19° __ 

 7.2! >S, 18°.5_ 

 7.276, 19°.4_ 

 7. 27'. i, 20° -. 

 7.284, 2#°.2_ 



Sb, Pb, 



7.214 



7.361 



7.432 



7.525 



7.622 



7.830 



8.330 



8.201, 13°.7. 



8.233 



8.953 



8.989, 11°. 7. 



8.999 



9.502 



Authority. 



Croockewitt. J. 1, 394. 

 Long. P. T. 1860, 177. 

 Calvert and Johnson. J. 12, 120. 

 Pillichody. J. 14, 279. 

 Riche. J. 15, 111. 

 Kupffer. Ann. (2), 40, 285. 

 Calvert and Johnson. J. 12, 120. 

 Pillichody. J. 14, 279. 

 Riche. J. 15, 111. 

 Kupffer. Ann. (2), 40 285. 

 Long. P. T. 1860, 177. 

 Calvert and Johnson. J. 12, 120. 

 Pillichody. J. 14, 279. 

 Calvert and Johnson. J. 12, 120. 

 Long. P. T. 1860, 177. 



Holzmann. P. T. 1860, 17' 



Long. P. T. 1860, 177. 



Riche. J. 15, 111. 



II u 



Calvert and Johnson. J. 12, 120. 



Riche. J. 15, 111. 

 Calvert and Johnson. 



J. 12, 120. 



Mattliiessen. P. T. 1860, 177. 

 Riche. J. 15, 111. 

 Calvert and Johnson. J. 12, 120 

 Matthiessen. P. T. 1860, 177. 

 Riche. J. 15, 111. 



